Electrolytic corrosion of iron by direct current
Post on 02-Jul-2016
Embed Size (px)
The JOURNAL OF THE
FRANKLIN INSTITUTE OF THE STATE OF PENNSYLVANIA
DEFOTED TO SCIENCE AND THE MECHANIC ART8
VoL. CLXXII OCTOBER, 191I No. 4
ELECTROLYT IC CORROSION OF IRON BY D IRECT CURRENT.
J. L. R. HAYDEN, Research Department, General Electric Company.
IN electric railways the rails are practically always used as return conductors. Since they are grounded, a part of the return current leaves the rails and passes through the ground, and if the voltage drop in the rails is considerable this stray cur- rent through the ground may be considerable and cause more or less serious corrosion of rails, gas and water pipes, iron structures and other metal parts located in the ground. The problem of studying the corrosion produced by stray direct currents in the ground, so as to reduce the damage caused by them to a min- imum, thus is Of great im~rtance.
This problem is frequently attacked by measuring the poten- tial difference between the different points of the rail return sys- tem and other metal parts in the ground, estimate therefrom the stray current, and from this judge on the amount of electrolytic corrosion which may be expected by Faraday's law. There is, however, some doubt, from the experience of electric railways, whether the passage of a stray current between metal parts in the ground necessarily involves corrosion in accordance with Faraday's law, or whether it may not be possible that currents
[NoTH.--The Franklin Institute is not responsible for the statements and opinions advanced by contributors to the JOURNAL.]
Copyright, t9z t, by THE FRANKLIN INSTITUTE. VOL. CLXXII, No. io3o~22 295
296 J . L .R . I-IAYDEN.
pass from metal to ground without corresponding corrosion of the metal.
As iron is the metal which is most frequently exposed and therefore of greatest importance, an investigation was started on the corrosion of iron under the influence of an electric current in Dr. Steinmetz's laboratory, and some preliminary results are given in the following:
The first electrolyte experimented with was a I per cent. solu- tion of ammonium nitrate, as nitrates and ammonia salts are the most probable conducting compounds in soils, especially in cities.
Sheet iron plates of 0.6 mm. thickness were used, carefully cleaned by hydrochloric and nitric acid and then mechanically. They were immersed in quart jars, each containing approxi- mately 800 cc. of electrolyte.
The plates dipped 9 cm. into the electrolyte. As negative were chosen plates of 14 cm. length, 5 cm. width,
giving 9 cm. 2 submerged surface. As positive were chosen plates of 14 cm. length and of differ-
ent widths, from 0.6 cm. to IO cm. The current was maintained constant, from a storage battery,
at .040 ampere, corresponding to current densities from 36 am- peres to 2.2 amperes per m 2.
After the test the plates were carefully cleaned with distilled water and chalk, and then weighed again.
In calculating the theoretical corrosion, the value of .29 mg. of iron per coulomb was used.
The duration of this test was 98 hours. The corrosion in no case approached the theoretical value,
but varied from one-tenth to one-third of the theoretical value, as follows :
In general, it was lower at higher current densities. Herefrom it seems to follow that it is not feasibte to estimate
the electrolytic corrosion of iron structures in the ground from the amount of stray current passing from these structures.
Current density, amperes per m ~ . . . . 36 18 9 4.5 2.25 Corrosion, per cent. of theoret ical .. lO.5 18.o 17.I 35.1 34.2
As the electrolytic corrosion of the iron was found much lower than the theoretical value, tests were made to see whether this is due to a partial corrosion, or due to periods in which no
ELECTROLYTIC CORROSION OF IRON. 297
corrosion takes place, that is, the iron is "passive," and to find the conditions under which the iron is passive, that is, does not corrode as positive terminal.
For this purpose, Io cells were made up, 8oo cm. 8 electrolyte, I per cent. solution of ammonium nitrate, with iron plates of 14 era. x 1.25 cm., dipping 9 cm. into the electrolyte, and operated in series, with 5o milliamperes of current, corresponding to a cur- rent density of about 22 amperes per m 2.
In two cells the plates were taken out, cleaned and weighed very frequently, in two cells less frequently, and in two cells left in continuously. In two cells the plates were put in the electrolyte one hour before the current was put on; two ceils were left with- out current and used to observe the spontaneous or chemical cor- rosion of the plates by the electrolyte.
In half the cells the electrolyte was changed after the cell had been running 24 hours; in the others the electrolyte was not changed.
The results of this and the following test are given in Table I, and some are plotted in Figure I.
It seems that there is no partial corrosion, but the iron is either passive, that is, practically no corrosion at 3.11 takes place, or the iron is active, that is, the full theoretical corrosion occurs. Fractional values of the theoretical corrosion are observed only where the cell has been operated continuously for a considerable time, and apparently had started ~/ctive and then become passive.
The average corrosion during the active periods is 49.6 mg. per hour, or, if counting only the shorter periods--during which a change of state is less probable---55.x rag. per hour, while the theoretical attack is 52.2 rag. per hour, and is shown by the dotted lines in Figure I.
The average chemical corrosion (without current) is 1.85 rag. per hour, or o.82 per m 2 an hour.
The corrosion of the anode during the active period thus is somewhat greater than the theoretical, as expected from chemical corrosion.
The average corrosion of the anode during the passive period is .2o rag. per hour, that is, less than % per cent. of the theoreti- cal, and is only about I I per cent. of the chemical corrosion. That is, the passage of a current from a passive anode protects the same from spontaneous or chemlcal corrosion.
298 ]. L. R. HAYDEN.
The average corrosion of the cathode was .4 rag. per hour with a pa,~sive anode, and .23 mg. per hour with an active anode.
I l ,J /
# i I
! I /
I / t I I p
I t I I ,, /z.//~ %/
/ / /
J ~ s // I / , f
p/ / f jt I , :~,
I / I / I i I i I
+, /Z"": / / I / ,,I )(/) I
i I d
#, # ~ It ( / . /
, / ,/#; ....//,/ /11 /
I1 / /
/ ii I
Electrolytic corrosion of iron by direct current. , % ammon. ~itrate solution, ~n amp. p. m2.
That is, if the anode is passive and does not corrode, the cathode corrodes about twice as much as if the anode is active and cor-
ELECTROLYTIC CORROSION OF IRON. 299
rodes. Even in this case, however, the corrosion of the cathode is only about 20 per cent. of the chemical corrosion, and about twice as much as that of the anode, b
It thus follows that during the passive state the corrosion of two iron plates is by the passage of the current reduced to a small fraction of the chemical corrosion. That is, under certain conditions (passive state), the passage of a direct current pro- tects both of the iron terminals between which it passes.
The active state occurred eight times. The passive state occurred ten times. Three times the corrosion was intermediate between that of
the active and the passive state. Of these, two were long con- tinuous runs, in which the behavior of the cells made a spon- taneous change from the active to the passive state probable.
Handling the plates, that is, taking them out, cleaning and weighing, frequently changes the state:
6 times from active to passive, 4 times from passive to active, 3 times the plate remained passive, Possibly I time the plate remained active.
Change of electrolyte changed
i time from passive to active, I time left the plates passive, I time probably left the plates active, I time probably changed from passive to active.
No definite effect of a change of the electrolyte on the state of the plates is thus shown. As at the end of the run the electro- lyte still gave the ammonia reaction and the nitric acid reaction, this is reasonable.
The voltage per cell was either low, about I volt, or high, 2. 7 volts, but intermediary voltages were observed only in two cases, at the end of a long active run, probably as the result of an increase of the resistance of the electrolyte.
The active state of corrosion was always accompanied by low voltage; the passive state, of no corrosion, by high voltage; and the voltage of the cell was found a good indicator of its state, and where a cell changed from active to passive state this was shown by the rise of voltage.
300 J . L .R . I-'IAYDEN.
The electrolyte and the deposit formed in the cell seem to give an indication of the state of the anode:
In all cells in which the anodes were passive at least during most of the time, and more particularly the latter part of the run, the electrolyte was clear, or only slightly yellow, and only little deposit was formed, of a yellow-brown color, apparently ferric hydrate.
In all cells in which the anodes were active and greatly corroded the electrolyte was very dirty, and masses of deposit formed. This deposit was of a dirty greenish-black color, indicating apparently ferrous hydrate.
Interesting was one cell in which active corrosion had taken place, but towards the end of the run the voltage had become high and